Maharashtra Engineering Maharashtra Engineering Research Institute, Nashik.Research Institute, Nashik.
WEL-COMES YOU !!!
MIX DESIGN OF MIX DESIGN OF ROLLER COMPACTED CONCR ETE ROLLER COMPACTED CONCR ETE
FOR FOR GHTAGHAR PROJECT GHTAGHAR PROJECT ––
A OVERVIEWA OVERVIEW
N. B. GhugeN. B. Ghuge V. B. Pandhare V. B. Pandhare C. L. NarkhedeC. L. Narkhede Director GeneralDirector General S. E. & Jt. Director S. E. & Jt. Director Sci. Research OfficerSci. Research Officer
Maharashtra Engineering Research Institute., NashikMaharashtra Engineering Research Institute., Nashik
GHATGHAR – A DEMONSTRATION
PROJECT • Ghatghar Pumped Storage Scheme is the first monument in the history of India, as a first project constructed with new concrete technology of RCC.
• It was taken up as Technical Demonstration Project by FAUP, New Delhi and Govt. of Maharashtra to demonstrate and understand the RCC and methodology of construction etc.
• Many agencies are associated for co-ordination, guidance, planning, design, research, construction etc. Efforts of Mr. Vimal Kumar, Director, FAUP has resulted in three RCC dams under Ghatghar Project.
• Govt. of Maharashtra has shown courage to do this experiment in Maharashtra giving opportunity to his officers to show their technical best.
• This was a team work and Chief Engineer, Koyna Project and his construction officers made it grand success with the help of other supporting agencies.
• RCC is very very different from conventional concrete. It is very sensitive to slight change in any of the properties of materials and ambient temperature. Construction technique is simple, but the methods should be followed sequentially.
RCC RCC -- A NEW CONCRETEA NEW CONCRETE
RCC is a zero slump concrete delivered by dumpers or conveyors, spread by bulldozers in horizontal layers and compacted by vibratory rollers in thin lifts- not exceeding 300mm to 600mm – from one abutment to other.
Concrete must be dry enough to support the weight of vibratory rollers and wet enough to permit distribution of paste throughout the mass.
Desired density is measured in-situ by Nuclear densometer and is achieved by adjusting no. of passes of vibratory rollers.
Construction is economical and rapid. Apart from these, RCC has high potential of large scale
utilization of fly ash whose safe disposal at present is a grave environmental concern.
Use of RCC has allowed many new dams in the world to become economically feasible at reduced cost and time realised from low cement and large fly ash content and rapid construction.
• MERI, Nashik was associated with this Project for
i) Testing of construction materials, right from water
to hardened concrete,
ii) Mix design of RCC
• MERI has done lot of mix designs in conventional concrete with and without use of fly ash.
• But this RCC concrete having no-slump (zero slump) consistency and compacted by vibratory rollers was new concrete to design.
•A workshop was organized to get acquainted with this technique
ROLE OF M.E.R.I., NASHIK
• A workshop on “Roller Compacted Concrete Dam” was organised in Nov. 1995 to understand RCC, construction and RCC dams for Research and Construction officers in India.
• Workshop was conducted by Mr. Ernest Schrader, an UNDP consultant.
• He visited the Ghatghar project site and gave technical specifications for laying of RCC, mix design, planning of the project, construction methodology etc.
Workshop on RCC
• Mr. Schrader gave guidance on basics of mix design to MERI, Nashik.
•Lessons were learnt and mix design methodology was developed in MERI, Nashik.
• He guided mix designs for Upper dam with low paste concrete and for Lower dam with high paste concrete.
• However, it was said that adoption of high paste RCC is best suited to Newcomers in this field and tropical countries like India. Low paste require patience and experience in RCC construction.
Mix Designs guided by Mr. Schrader (12/1996 – 10/1998)
36 MIX DESIGNS FOR UPPER DAM
• Cementitious content : 80 & 150 kg/cum
• Cement : 43 grade cement
• Fly ash : Nashik TPS
• Coarse aggregate : 40-20, 20-5mm from Lower dam site
• Fine aggregate : 25% natural sand + 75% crushed
• stone sand.
• Mixes were carried out as directed by the Consultant with following proportions and tested up to 365 days for various properties such as density, compressive strength, spilt tensile strength, Young Modulus, permeability etc.
i) For cementitious content 150 kg/cum. • 50% fly ash with varying water contents
[ Optimum (70 lit) ± 0.4% & 0.8% ]. • 50% fly ash with addition of Stone dust fines
at 3% & 6%.
ii) For cementitious content 80 kg/cum.
• 30%, 50%, & 70% fly ash substitution. • 50% fly ash with varying water contents. • 50% fly ash with varying Stone dust fines. • 50% fly ash with addition of admixture.
( 0.4% to 1.6%)
30 MIX DESIGNS
FOR LOWER DAM
Mix designs were carried out for 115, 150, 185 and 220 kg/cum cementitious content.
i) For c. c. 115 & 185 kg/cum. • 30%, 50% & 70% fly ash
ii) For c.c. 150 kg/cum • 30%, 50% & 70% fly ash • 30%, 50% & 70% fly ash with varying water content iii) For c. c. 200 kg/cum • 30%, 50% & 70% fly ash • 50% fly ash with addition of stone dust fines. • 50% fly ash with admixture
MIX DESIGNS BY EPDCIL, JAPAN (10/1998 – 12/2000)
ELECTRIC POWER DEVELOPMENT CO. INTERNATIONAL LTD (EPDCIL), Japan was appointed as new consultant who has large experience in building of RCC dams in Japan.
EPDCIL has abandoned the mix designs of Mr. Schrader and set the parameters for mix design as • High paste RCC • Layered construction with monoliths. •GEVR concrete membrane of 2m width @ U/P & D/P side ends. • 50 MSA aggregate & 100% crushed sand. • Cohesive mix without segregation. • 150 kg/cm2 compressive strength at 90 days age. • Density more than 2.5 T/cum. • Satisfactory impermeability .
OBJECTIVES SET FOR MIX DESIGN
• Optimize the gradation of the aggregates with maximum size of aggregate.
• Optimize the workability and define the water content for the RCC mix.
• Define minimum cementitious content commensurate with cohesive mix.
• Optimize fly ash content to get desired results.
PARAMETERS FIXED BY EPDCIL, JAPAN
• Optimum crushed sand : 35% by weight of the total aggregate.
• MSA of Aggregate : 53mm • Coarse aggregate : 50-20mm, 20-10mm and 10-5mm • Optimum workability : Ve Be time of 25 sec. • Water content : initially 115 lit/cum. • Fly ash substitution : from 30% to 70% by weight of the
cementitious content. • Fly ash : Nashik thermal Power Station, Nashik. • Cementitious content : 220 kg/cum • Grade of cement : 43 grade. • Admixture : PLASTIMENT–R admixture • Dose of admixture : 0.88% by weight of cementitious
material fixed on laboratory trials
• Gradation of coarse aggregate: Aggregates were internally proportioned for various percentage combinations to achieve maximum dry rodded density to get minimum voids and dense concrete as suggested by EPDCIL .
•The overall gradation of 50-20 : 20-10 : 10-5mm aggregate arrived at proportion 52 :26.40 : 21.60
• 23 Mixes were conducted for c.c. 200 kg/cum with 30% to 70% fly ash substitution and various properties were observed up to 365 days.
Workability is measured by Ve Be Apparatus.
Concrete is placed in cylindrical jar of 23 cm diameter by 23 cm height. Round metal weight of 10kg is placed on the concrete and vibrated until the cement slurry comes out around the weight. This indicates that the concrete is fully compacted and additional remaining slurry comes out. The time elapsed is called as Ve Be time, which is the measure of workability. Instrument will be shown in the photographs at end of narration
For a good RCC mix, this time shall be 25 to 30 seconds.
Conclusions of EPDCIL mixes
• Ve Be time observed in the range of 25 to 30 sec indicating cohesive mix.
• Density was more than desired 2.5 T/cum.
• Modulus of Elasticity comparable to conventional concrete.
• All specimen gave compressive strength more than the desired value 150 kg/cm2.
• Permeability of all specimen was satisfactory.
CONSULTATION WITH M D & A, UK
• EPDCIL consulted Malcolm Dunstan & Associates of UK and as per his suggestion, 17 additional mixes for
cementitious contents 180, 200, 220 & 240 kg/cum and
40% to 70% fly ash substitution
were carried out and test results are as follows.
• He suggested to adopt design age of 180 days at proto as structure will not fully loaded
Click here to load reader